6.2.2 Solidification and the Art of Casting
|That was that pressing question on the back of your mind! Or was it? Why should this be a pressing question? You know what happens when we go from the liquid phase to whatever solid phase: the stuff solidifies!|
|Indeedbut how? If you look at our
iron-carbon phase diagram again and
stay right with the 1,3 % carbon composition line we used before, you realize
that upon cooling from the liquid ("L") state you run through
several phasefields before you are at room temperature:
|To put the question in other words: You and about
everybody else too, has a far too naive view of what is implied in
casting something. Ask around and you will find
|Let's say the melt consists of iron and 1.3 % carbon. Almost everybody out there would expect that upon "freezing" you get solid iron with 1.3 % carbon "somehow" dissolved in it. Almost nobody would guess that at room temperature you have rather pure iron with some embedded iron carbide but that at higher temperatures the solid would be completely different from that.|
|Nobody (well, almost nobody) would guess that the
science of casting is a rather complex
I grant that you, the ancient smith, did not cast sword blades or anything else made from pure iron or steel. So why should you worry? Because in order to understand wootz steel, we need to look at what really happens when we go from the liquid phase to a two phase region! We will find that the basic difference between wootz steel blades and all others stems from the fact that wootz steel was liquid once.
|Of course, all we need to do is to
learn a few more things about phase diagrams. Then we give the iron-carbon
phase diagram a close look and figure out what happens when we go from the
liquid phase to the solid phases. It should contain that information, after
all. It does, indeed, but the iron-carbon phase diagram is also a rather
complex one. You might wonder if most of the other »8.000 binary phase diagrams are much simpler? Maybe
only iron and carbon produce such a complicated mess?
The squiggly lines "»", by the way, mean simply "about". I'm going to use common science abbreviations more often from now on because at this point the faint of heart or soft of brain are no longer with me.
|So does the iron-carbon
phase diagram belong to the more complex ones?
Unfortunately or luckily, depending on your point of view, this is not the case. There are plenty of phase diagrams out there that are far more complicated than the iron-carbon one; take, for example the phase diagrams for copper (Cu) and tin (Sn), producing what we call bronze, or copper (Cu) and zinc (Zn), producing what we call brass. They are shown in an illustration module. Both phase diagrams plus plenty of others are easily found in the Internet.
If you start to feel sorry for our students, consider that this will give them jobs. Having a lot of complicated phase diagrams is actually good luck because it will give us opportunities for engineering novel and useful materials for a long time to come.
Simple phase diagrams are not only intellectually boring, there is just not much you can do with those materials.
|Fortunately for you,
there are simpler phase diagrams, too, and they make it easier to get the point
across that I want to make now.
Examples for most simple phase diagrams include the gold - silver, or copper - nickel systems. Here we give a quick look at a slightly more complicated phase diagram: a mixture of lead (Pb) and tin (Sn), including common solder.
|Let's start with a composition around
73 % tin (Sn) (the green state point in the figure above). Cool this mixture
down and it will solidify directly from the
melt at the "eutectic point" into
a two-phase solid. It will not go through a
phase field where it decomposes into a mixture of liquid and solid with
as we had
before. The solid thus has exactly the same
composition as that of the melt. It decomposes into two different
phases (a and
b in the example above) but the composition is the
same as the melt.
That's what the phase diagram tells you. As you can also see, the eutectic composition that we have at an eutectic point is by necessity the composition with the lowest possible melting point of a binary system.
|Now you realize why "eutectic" is such a magic word in working
metals! If there is an eutectic composition
in your phase diagram, it makes for easy
|"Eutectic", by the way, is from ancient Greek and means: "easily melted". Aha!|
|To be sure, the solid just below the
eutectic point does decompose into tin-rich lead and almost pure tin as shown
in the phase diagram. But the over-all
composition is unchanged.
What a typical eutectic microstructure looks like is shown in the following picture:
|Two things are obvious:
|What you realize by now is that solidification in general and casting in particular is not as simple as it looks, indeed.||
|Let's look now at non-eutectic compositions, for example the
red composition at about 33 % tin as
shown above and on the right. The melt,
according to the phase diagram, decomposes into some lead-rich solid stuff and
a tin-rich liquid as shown exemplary by the two red state points in the L +
a phase field.
By the time when the last droplet of the remaining tin-rich liquid has solidified, the solid has a very inhomogeneous over-all composition as shown below.
This is nothing new. When you freeze the binary system H2O - NaCl (also known as salty water), the first solid that crystallizes from the "melt" is sweet ice that contains very little salt. The more ice you form, the saltier the water must get. The last bit of water to solidify then must contain all the salt and that ice then is salty. Your ice, in other words, is not uniform with respect to its saltiness.
If you don't believe me, look up this illustration module.
|But back to the Pb - Sn system. The chunks
crystallizing first are lead-rich compared to the over-all composition; the
remaining liquid then is enriched in tin.
Now comes the crucial questions
|No, no, no!!! Not at all! Consider:
|As the temperature goes down, more and more liquid crystallizes and the newly crystallized parts get increasingly tin-rich. The final result is a lump of lead-tin alloy that is lead-rich on the outside and tin-rich in the inside relative to its gross composition. Schematically, it looks like this:|
|We have now encountered the phenomenon of segregation, meaning that the composition of the solid material is not the same everywhere (as you probably would have liked it to be). It varies considerably on a "macroscopic" scale, like from the outside to the inside of the crucible or die that is used for solidification. If we just describe what we get, we say that the components of our mixture got segregated or separated. And what that means is:|
|Even worse, besides this more "macroscopic" segregation that leads to variations in the composition of the solid on a large scale, there is also something called "micro segregation" on a small scale. This is shown below for our example from above|
|On the left the variation of the lead and tin concentration due to macro segregation, coming right from the phase diagram, is shown schematically. On the right we look at just the lead concentration in a small region (millimeter or smaller) The concentration fluctuates more or less periodically, due to micro segregation effects, around the average values (dotted line) given by macro segregation.|
|Micro segregation results from reasons not contained in the "nirvana" phase diagram. We will give it a closer look because it is directly responsible for the "water" structure of wootz steel blades.|
| So you better get used to the term
segregation. It is is a key phenomenon for
sword making (and for most everything else).
In human affairs segregation is usually considered to be bad. In Materials Science affairs, segregation is neutral.
From the viewpoint of the material, macro segregation is good because it brings the system closer to nirvana. And everybody is entitled to pursue happiness, after all.
From the viewpoint of the Materials Engineer, segregation is often bad. However, you couldn't make wootz blades without it, so for this purpose it is good. It is also great if you want to clean your material. If you want sweet ice from water contaminated with salt, let if freeze and take only the parts that froze first. They are clean. The same principle applies of you want extremely clean silicon, and so on.
|Nothing helps, you need to understand at least the basics of macro- and micro segregation because we need to manipulate that behavior quite a bit to make sword blades. If we deal with segregation the right way it will not bother us too much anymore, and we might even use it to our advantage like in wootz steel. I will give you some hints here, use the science module if you want to learn (a lot) more.|
|We already know that
macro segregation is a direct consequence
of a phase diagram, which in turn is a direct consequence of the second
So let's now give a first quick look at some of those many new things that might cause micro segregation.
|When I introduced you to
we looked at solidification at some solid - liquid boundaries advancing into
the material from various nucleation points typically found at the surface of
the container. Look at the
figure once more to recall what I mean. Now notice that the way it is drawn
is far too simple with respect to reality.
In the figure above parts of the old figure are shown once more. If we would look a bit closer at one of the growing crystals like the yellow one, it would often look like the "dendrite" shown above.
|Dendritic or "tree-like" growth is
fairly common whenever the "driving
forces" are large (I'll come to that). For the time being, just
note that you have large "driving
forces" when you cool down quickly.
What happens then is fairly complex, if well understood. I'll give you details later. In essence the solidifying part releases "heat of solidification" and thus heats up itself plus the liquid around it. That makes solidification more difficult and slows down the advancement of the dendrite tip into the liquid.
|Heat of solidification is simply the
energy no longer needed if the atoms don't run around in the liquid anymore. As
soon as we have a solid, the atoms are tied down to a place in the crystal
lattice where they can only vibrate so much. We
You know that effect quite well, you just didn't give it fancy names. Put some very cold water close to the freezing point into your freezer. It won't freeze instantly because the energy released as "heat of solidification" heats it up again. Your freezer must transport this energy to the outside world, and that takes a while.
Same thing in reverse. Put your frozen soup into a pot and put it on your range going at full blast. It will not liquefy instantly; it actually takes quite some time. Now you have to supply the heat of solidification or the heat of melting, same thing, and that takes a while.
|We already have a first reason why solidification could be a stop-and-go process even for pure materials. Let's say the solid-liquid phase boundary advances rapidly into the liquid part at some time. Then a lot of heat of solidification is produced, the temperature goes up and things slow down. Now less heat of solidification is produced, the temperature goes down, and things speed up once more. And so on.|
|If the melt contains any impurities, things get more complicated. Impurities usually like it better in the liquid (look at the phase diagrams!) so the solid will have a lower concentration at first. A heat of steel always contains all kind of impurities, so solidifying steel is always rather complicated from a segregation point of view.|
|The liquid close to the solid-liquid
phase boundary thus will get impurity-richer because it "get's" all
impurities not accepted by the solid. The impurity concentration close to the
the solid-liquid boundary is thus larger than it ought to be. That always means
that the local melting point is now lower
than it ought to be. This makes solidification more difficult, it slows down or
comes to a stop.
Meanwhile, the surplus impurities in the melt diffuse into the bulk of the melt and their concentration close to the solid-liquid phase boundary goes down. That means the local melting point goes up, and solidification speeds up.
Once more, good reasons for a stop-and-go process of solidification or, to put it more precisely, a fluctuating growth speed of the solid.
|To summarize and generalize: There are reasons why the solid-liquid boundary should not advance with constant speed into the liquid. In other words, there are reasons why the growth speed of the interface should fluctuate or oscillate. There are also reasons why this should not happen in lock step everywhere but in different ways at different places.|
|Be that as it may, the decisive parameter in the end is the (local) growth speed, meaning how fast the solid-liquid interface advances into the liquid. The reason for that is simple: How much impurities are incorporated into the solid depends on that growth speed.|
|You should protest here and tell me that how much of an impurity end up in a solid depends on the phase diagram and nothing else! It should thus not depend on the growth speed of the interface!|
|You are right! And I'm right, too. We both can be right about a mutually exclusive item because, as I stated long before, "Phase diagrams show only the "nirvana" state". A freshly solidified piece of material may not be in that desirable state, however!|
|Looking at this a bit more closely (with equations), it turns out that the phases predicted in the phase diagram will only come into their ideal being if the solid-liquid boundary advances v e r y s l o w l y. If it advances with normal speed, the expelled impurity atoms close the solid-liquid boundary do not have enough time to move away from the boundary into the depth of the liquid. What then solidifies next is a liquid different from that in the phase diagram. You will now incorporate more impurities in the growing crystal.|
|That's sounds more complicated than it really is. All it means is that the fraction of impurities ending up in the crystal relative to those in the melt goes up with increasing growth rate. Keeping this in mind, let's see what happens now if we solidify a melt containing two kinds of atoms.|
|Let's assume that we have some fast crystallization at the solid-liquid interface of some growing grain. We have already seen that several things conspire to cause the growth rate to fluctuate or oscillate, meaning that crystallization happens in a stop-and-go fashion. Let's look at this again but now also keeping in mind the impurity incorporation into the crystal:|
|OK - I admit that the phenomenon of
constitutional supercooling is
a bit hard to understand when first encountered. It is even hard to calculate if we look at it in three dimensions and
not just one-dimensionally as implicitly done in the prose above.
In the final result, however, it is quite likely that the sold-liquid interface moves in a stop-and-go fashion in not just one but in all three dimensions. This produces not only the characteristic dendritic shapes but also a more or less periodic variation of the impurity concentration in the solid.
| Here is the reason for all kinds of
what we call "pattern
formation" in solid materials, and that includes the patterns
found in wootz steel. We like that pattern
and see it as aesthetically pleasing and a sign of quality.
It also includes pattern we find in the ultra-pure silicon (Si) crystals we use for making chips. We hate those patterns but must live with them. More about that in the science link.
Segregation is rather the rule and not the exception when you solidify liquids. We will look at this some more in later chapters.
|Pattern formation by segregation effects comes with many names. They may be called "banding", or "striation" and always involve a non-uniform distribution of impurities. Of course, the effects of segregation have been observed and described centuries before they were understood.|
|Sorry. I now destroyed your naive view that solidification and casting is a simple process. Just pure some liquid into the mold, wait a while, and take out the solid product? Ha!|
|1)||S.A. David, S.S. Babu, and J.M. Vitek; "Welding: Solidification and Microstructure", JOM (2003) p. 14. By kind permission of S.A. David|
© H. Föll (Iron, Steel and Swords script)